#------------------------------------------------------------------------------
#$Date: 2019-12-26 22:24:51 +0200 (Thu, 26 Dec 2019) $
#$Revision: 246182 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/31/19/2311947.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2311947
loop_
_publ_author_name
'Spiridonova, Tatyana S.'
'Solodovnikov, Sergey F.'
'Savina, Aleksandra A.'
'Solodovnikova, Zoya A.'
'Stefanovich, Sergey Yu'
'Lazoryak, Bogdan I.'
'Korolkov, Iliya V.'
'Khaikina, Elena G.'
_publ_section_title
;
 Synthesis, crystal structures and properties of the new compounds
 K₇₋ₓAg₁₊ₓ(XO₄)₄ (X = Mo, W).
;
_journal_coeditor_code           LY3055
_journal_issue                   'Pt 12'
_journal_name_full
'Acta crystallographica. Section C, Structural chemistry'
_journal_page_first              1071
_journal_page_last               1077
_journal_paper_doi               10.1107/S2053229617015674
_journal_volume                  73
_journal_year                    2017
_chemical_formula_iupac          'K6.68 Ag1.32 Mo4 O16'
_chemical_formula_moiety         'Ag1.32 Mo4 O16, 6.68(K)'
_chemical_formula_sum            'Ag1.32 K6.68 Mo4 O16'
_chemical_formula_weight         1043.34
_chemical_name_systematic
;
Heptapotassium silver tetrakis(tetraoxomolybdate)
;
_space_group_IT_number           186
_space_group_name_Hall           'P 6c -2c'
_space_group_name_H-M_alt        'P 63 m c'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_atom_sites_solution_hydrogens   other
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   12.4188(2)
_cell_length_b                   12.4188(2)
_cell_length_c                   7.4338(2)
_cell_measurement_reflns_used    9592
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      31.535
_cell_measurement_theta_min      3.789
_cell_volume                     992.89(3)
_computing_cell_refinement
;
SAINT (Bruker, 2004)
;
_computing_data_collection
;
APEX2 (Bruker, 2004)
;
_computing_data_reduction
;
SAINT (Bruker, 2004)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 2008)
;
_computing_publication_material
;
SHELXL2017 (Sheldrick, 2015)
;
_computing_structure_refinement
;
SHELXL2017 (Sheldrick, 2015)
;
_computing_structure_solution
;
SHELXS97 (Sheldrick, 2008)
;
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean 25
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Bruker--Nonius X8 APEX CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0332
_diffrn_reflns_av_sigmaI/netI    0.0194
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            9592
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.535
_diffrn_reflns_theta_min         3.789
_diffrn_standards_decay_%        0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    5.199
_exptl_absorpt_correction_T_max  0.455
_exptl_absorpt_correction_T_min  0.356
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(SADABS; Bruker, 2004)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.490
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       fragment
_exptl_crystal_F_000             969.8
_exptl_crystal_size_max          0.250
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.180
_refine_diff_density_max         1.401
_refine_diff_density_min         -1.310
_refine_ls_abs_structure_details
;
Refined as an inversion twin
;
_refine_ls_abs_structure_Flack   0.15(8)
_refine_ls_goodness_of_fit_ref   1.120
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     65
_refine_ls_number_reflns         1189
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.120
_refine_ls_R_factor_all          0.0181
_refine_ls_R_factor_gt           0.0179
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+2.0336P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0402
_refine_ls_wR_factor_ref         0.0403
_reflns_number_gt                1178
_reflns_number_total             1189
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ly3055sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        992.89(4)
_cod_database_code               2311947
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z+1/2'
'x-y, -y, z+1/2'
'-x, -x+y, z+1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
Mo Mo1 0.333333 0.666667 0.2815(3) 0.01895(17) Uani d 1
Mo Mo2 0.33981(4) 0.16990(2) 0.1711(3) 0.01329(9) Uani d 1
K K1 0.000000 0.000000 0.000000 0.0188(4) Uani d 1
K K2 0.17108(6) 0.34216(13) 0.1756(4) 0.0251(2) Uani d 1
K K3 0.5161(4) 0.4839(4) 0.3916(8) 0.0254(6) Uani d 0.894(5)
Ag Ag1 0.666667 0.333333 0.3296(3) 0.0274(2) Uani d 1
Ag Ag2 0.5074(12) 0.4926(12) 0.428(4) 0.055(8) Uani d 0.106(5)
O O1 0.333333 0.666667 0.522(2) 0.079(5) Uani d 1
O O2 0.4100(2) 0.5900(2) 0.2003(8) 0.0345(11) Uani d 1
O O3 0.3559(4) 0.2931(4) 0.0376(7) 0.0450(9) Uani d 1
O O4 0.1885(4) 0.0943(2) 0.2621(7) 0.0339(10) Uani d 1
O O5 0.4512(4) 0.22559(18) 0.3471(7) 0.0308(9) Uani d 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O2 Mo1 O2 . 3_565 108.84(19)
O2 Mo1 O2 . 2_665 108.84(19)
O2 Mo1 O2 3_565 2_665 108.83(19)
O2 Mo1 O1 . . 110.10(19)
O2 Mo1 O1 3_565 . 110.10(19)
O2 Mo1 O1 2_665 . 110.10(19)
O2 Mo1 Ag1 . 4_664 69.90(19)
O2 Mo1 Ag1 3_565 4_664 69.90(19)
O2 Mo1 Ag1 2_665 4_664 69.90(19)
O1 Mo1 Ag1 . 4_664 180.0
O2 Mo1 K2 . 3_565 147.2(2)
O2 Mo1 K2 3_565 3_565 57.746(17)
O2 Mo1 K2 2_665 3_565 57.746(18)
O1 Mo1 K2 . 3_565 102.71(5)
Ag1 Mo1 K2 4_664 3_565 77.29(5)
O2 Mo1 K2 . 2_665 57.747(18)
O2 Mo1 K2 3_565 2_665 147.2(2)
O2 Mo1 K2 2_665 2_665 57.749(18)
O1 Mo1 K2 . 2_665 102.71(5)
Ag1 Mo1 K2 4_664 2_665 77.29(5)
K2 Mo1 K2 3_565 2_665 115.30(4)
O2 Mo1 K2 . . 57.747(18)
O2 Mo1 K2 3_565 . 57.749(18)
O2 Mo1 K2 2_665 . 147.2(2)
O1 Mo1 K2 . . 102.71(5)
Ag1 Mo1 K2 4_664 . 77.29(5)
K2 Mo1 K2 3_565 . 115.30(4)
K2 Mo1 K2 2_665 . 115.30(4)
O2 Mo1 Ag2 . 2_665 123.16(10)
O2 Mo1 Ag2 3_565 2_665 123.16(9)
O2 Mo1 Ag2 2_665 2_665 36.4(4)
O1 Mo1 Ag2 . 2_665 73.7(4)
Ag1 Mo1 Ag2 4_664 2_665 106.3(4)
K2 Mo1 Ag2 3_565 2_665 66.01(14)
K2 Mo1 Ag2 2_665 2_665 66.01(15)
K2 Mo1 Ag2 . 2_665 176.4(4)
O2 Mo1 Ag2 . 3_565 123.16(10)
O2 Mo1 Ag2 3_565 3_565 36.4(4)
O2 Mo1 Ag2 2_665 3_565 123.16(10)
O1 Mo1 Ag2 . 3_565 73.7(4)
Ag1 Mo1 Ag2 4_664 3_565 106.3(4)
K2 Mo1 Ag2 3_565 3_565 66.01(15)
K2 Mo1 Ag2 2_665 3_565 176.4(4)
K2 Mo1 Ag2 . 3_565 66.01(15)
Ag2 Mo1 Ag2 2_665 3_565 112.5(3)
O2 Mo1 Ag2 . . 36.4(4)
O2 Mo1 Ag2 3_565 . 123.16(10)
O2 Mo1 Ag2 2_665 . 123.16(10)
O1 Mo1 Ag2 . . 73.7(4)
Ag1 Mo1 Ag2 4_664 . 106.3(4)
K2 Mo1 Ag2 3_565 . 176.4(4)
K2 Mo1 Ag2 2_665 . 66.01(15)
K2 Mo1 Ag2 . . 66.01(14)
Ag2 Mo1 Ag2 2_665 . 112.5(3)
Ag2 Mo1 Ag2 3_565 . 112.5(3)
O2 Mo1 K3 . 2_665 121.99(3)
O2 Mo1 K3 3_565 2_665 121.99(3)
O2 Mo1 K3 2_665 2_665 31.9(2)
O1 Mo1 K3 . 2_665 78.24(9)
Ag1 Mo1 K3 4_664 2_665 101.76(9)
K2 Mo1 K3 3_565 2_665 64.36(3)
K2 Mo1 K3 2_665 2_665 64.36(3)
K2 Mo1 K3 . 2_665 179.05(11)
Ag2 Mo1 K3 2_665 2_665 4.5(4)
Ag2 Mo1 K3 3_565 2_665 114.38(12)
Ag2 Mo1 K3 . 2_665 114.38(12)
O3 Mo2 O3 9 . 109.7(3)
O3 Mo2 O4 9 . 108.00(14)
O3 Mo2 O4 . . 108.00(14)
O3 Mo2 O5 9 . 110.59(17)
O3 Mo2 O5 . . 110.59(17)
O4 Mo2 O5 . . 109.9(2)
O3 Mo2 K2 9 3 48.97(14)
O3 Mo2 K2 . 3 139.87(17)
O4 Mo2 K2 . 3 62.59(5)
O5 Mo2 K2 . 3 109.11(7)
O3 Mo2 K2 9 . 139.87(17)
O3 Mo2 K2 . . 48.97(14)
O4 Mo2 K2 . . 62.59(5)
O5 Mo2 K2 . . 109.11(7)
K2 Mo2 K2 3 . 120.68(4)
O3 Mo2 K2 9 5_554 55.40(17)
O3 Mo2 K2 . 5_554 55.40(17)
O4 Mo2 K2 . 5_554 112.99(17)
O5 Mo2 K2 . 5_554 137.14(15)
K2 Mo2 K2 3 5_554 90.72(5)
K2 Mo2 K2 . 5_554 90.72(5)
O3 Mo2 Ag1 9 . 94.97(14)
O3 Mo2 Ag1 . . 94.97(14)
O4 Mo2 Ag1 . . 138.87(17)
O5 Mo2 Ag1 . . 29.00(15)
K2 Mo2 Ag1 3 . 117.79(2)
K2 Mo2 Ag1 . . 117.79(2)
K2 Mo2 Ag1 5_554 . 108.14(3)
O3 Mo2 K2 9 5 124.50(17)
O3 Mo2 K2 . 5 124.50(17)
O4 Mo2 K2 . 5 67.79(17)
O5 Mo2 K2 . 5 42.08(15)
K2 Mo2 K2 3 5 89.67(5)
K2 Mo2 K2 . 5 89.67(5)
K2 Mo2 K2 5_554 5 179.22(5)
Ag1 Mo2 K2 . 5 71.08(3)
O3 Mo2 K3 9 2_655 65.7(2)
O3 Mo2 K3 . 2_655 143.81(15)
O4 Mo2 K3 . 2_655 107.34(14)
O5 Mo2 K3 . 2_655 48.56(11)
K2 Mo2 K3 3 2_655 66.27(11)
K2 Mo2 K3 . 2_655 153.30(11)
K2 Mo2 K3 5_554 2_655 115.61(9)
Ag1 Mo2 K3 . 2_655 51.94(10)
K2 Mo2 K3 5 2_655 63.95(9)
O3 Mo2 K3 9 . 143.81(15)
O3 Mo2 K3 . . 65.7(2)
O4 Mo2 K3 . . 107.34(14)
O5 Mo2 K3 . . 48.56(11)
K2 Mo2 K3 3 . 153.30(11)
K2 Mo2 K3 . . 66.27(11)
K2 Mo2 K3 5_554 . 115.61(9)
Ag1 Mo2 K3 . . 51.94(11)
K2 Mo2 K3 5 . 63.95(9)
K3 Mo2 K3 2_655 . 96.4(2)
O3 Mo2 K1 9 . 84.65(14)
O3 Mo2 K1 . . 84.65(14)
O4 Mo2 K1 . . 41.78(17)
O5 Mo2 K1 . . 151.66(15)
K2 Mo2 K1 3 . 62.34(2)
K2 Mo2 K1 . . 62.34(2)
K2 Mo2 K1 5_554 . 71.21(4)
Ag1 Mo2 K1 . . 179.35(3)
K2 Mo2 K1 5 . 109.57(4)
K3 Mo2 K1 2_655 . 128.27(11)
K3 Mo2 K1 . . 128.27(11)
O4 K1 O4 4_554 6_554 81.50(16)
O4 K1 O4 4_554 5_554 81.50(16)
O4 K1 O4 6_554 5_554 81.50(16)
O4 K1 O4 4_554 3 100.58(9)
O4 K1 O4 6_554 3 177.23(17)
O4 K1 O4 5_554 3 100.58(9)
O4 K1 O4 4_554 . 177.23(17)
O4 K1 O4 6_554 . 100.58(9)
O4 K1 O4 5_554 . 100.58(9)
O4 K1 O4 3 . 77.28(15)
O4 K1 O4 4_554 2 100.58(9)
O4 K1 O4 6_554 2 100.58(9)
O4 K1 O4 5_554 2 177.23(17)
O4 K1 O4 3 2 77.28(15)
O4 K1 O4 . 2 77.28(15)
O4 K1 K1 4_554 4_554 48.91(11)
O4 K1 K1 6_554 4_554 48.91(11)
O4 K1 K1 5_554 4_554 48.91(11)
O4 K1 K1 3 4_554 133.86(10)
O4 K1 K1 . 4_554 133.86(10)
O4 K1 K1 2 4_554 133.86(10)
O4 K1 K1 4_554 4 131.09(11)
O4 K1 K1 6_554 4 131.09(11)
O4 K1 K1 5_554 4 131.09(11)
O4 K1 K1 3 4 46.14(10)
O4 K1 K1 . 4 46.14(10)
O4 K1 K1 2 4 46.14(10)
K1 K1 K1 4_554 4 180.0
O4 K1 Mo2 4_554 3 81.95(6)
O4 K1 Mo2 6_554 3 158.10(12)
O4 K1 Mo2 5_554 3 81.96(6)
O4 K1 Mo2 3 3 24.67(9)
O4 K1 Mo2 . 3 96.48(6)
O4 K1 Mo2 2 3 96.48(6)
K1 K1 Mo2 4_554 3 109.19(3)
K1 K1 Mo2 4 3 70.81(3)
O4 K1 Mo2 4_554 . 158.10(12)
O4 K1 Mo2 6_554 . 81.95(6)
O4 K1 Mo2 5_554 . 81.95(6)
O4 K1 Mo2 3 . 96.48(6)
O4 K1 Mo2 . . 24.67(9)
O4 K1 Mo2 2 . 96.48(6)
K1 K1 Mo2 4_554 . 109.19(3)
K1 K1 Mo2 4 . 70.81(3)
Mo2 K1 Mo2 3 . 109.76(3)
O4 K1 Mo2 4_554 2 81.96(6)
O4 K1 Mo2 6_554 2 81.96(6)
O4 K1 Mo2 5_554 2 158.10(12)
O4 K1 Mo2 3 2 96.47(6)
O4 K1 Mo2 . 2 96.48(6)
O4 K1 Mo2 2 2 24.67(9)
K1 K1 Mo2 4_554 2 109.19(3)
K1 K1 Mo2 4 2 70.81(3)
Mo2 K1 Mo2 3 2 109.75(3)
Mo2 K1 Mo2 . 2 109.76(3)
O4 K1 K2 4_554 . 125.09(3)
O4 K1 K2 6_554 . 60.62(11)
O4 K1 K2 5_554 . 125.09(3)
O4 K1 K2 3 . 116.61(11)
O4 K1 K2 . . 55.15(3)
O4 K1 K2 2 . 55.15(3)
K1 K1 K2 4_554 . 109.53(4)
K1 K1 K2 4 . 70.47(4)
Mo2 K1 K2 3 . 141.28(6)
Mo2 K1 K2 . . 56.295(12)
Mo2 K1 K2 2 . 56.295(12)
O4 K1 K2 4_554 2 60.62(11)
O4 K1 K2 6_554 2 125.09(3)
O4 K1 K2 5_554 2 125.09(3)
O4 K1 K2 3 2 55.15(3)
O4 K1 K2 . 2 116.61(11)
O4 K1 K2 2 2 55.15(3)
K1 K1 K2 4_554 2 109.53(4)
K1 K1 K2 4 2 70.47(4)
Mo2 K1 K2 3 2 56.294(12)
Mo2 K1 K2 . 2 141.28(6)
Mo2 K1 K2 2 2 56.295(12)
K2 K1 K2 . 2 109.41(4)
O4 K1 K2 4_554 3 125.09(3)
O4 K1 K2 6_554 3 125.09(3)
O4 K1 K2 5_554 3 60.62(11)
O4 K1 K2 3 3 55.15(3)
O4 K1 K2 . 3 55.15(3)
O4 K1 K2 2 3 116.61(11)
K1 K1 K2 4_554 3 109.53(4)
K1 K1 K2 4 3 70.47(4)
Mo2 K1 K2 3 3 56.295(12)
Mo2 K1 K2 . 3 56.295(12)
Mo2 K1 K2 2 3 141.29(6)
K2 K1 K2 . 3 109.41(4)
K2 K1 K2 2 3 109.41(4)
O4 K1 K2 4_554 4_554 47.51(3)
O4 K1 K2 6_554 4_554 105.67(12)
O4 K1 K2 5_554 4_554 47.51(3)
O4 K1 K2 3 4_554 77.10(10)
O4 K1 K2 . 4_554 132.95(2)
O4 K1 K2 2 4_554 132.95(2)
K1 K1 K2 4_554 4_554 56.76(4)
K1 K1 K2 4 4_554 123.24(4)
Mo2 K1 K2 3 4_554 52.42(3)
Mo2 K1 K2 . 4_554 125.107(14)
Mo2 K1 K2 2 4_554 125.107(14)
K2 K1 K2 . 4_554 166.29(8)
K2 K1 K2 2 4_554 77.824(15)
K2 K1 K2 3 4_554 77.825(15)
O4 K1 K2 4_554 6_554 47.51(3)
O4 K1 K2 6_554 6_554 47.51(3)
O4 K1 K2 5_554 6_554 105.68(12)
O4 K1 K2 3 6_554 132.95(2)
O4 K1 K2 . 6_554 132.95(2)
O4 K1 K2 2 6_554 77.10(10)
K1 K1 K2 4_554 6_554 56.76(4)
K1 K1 K2 4 6_554 123.24(4)
Mo2 K1 K2 3 6_554 125.106(14)
Mo2 K1 K2 . 6_554 125.107(14)
Mo2 K1 K2 2 6_554 52.42(3)
K2 K1 K2 . 6_554 77.824(15)
K2 K1 K2 2 6_554 77.824(15)
K2 K1 K2 3 6_554 166.29(8)
K2 K1 K2 4_554 6_554 92.83(5)
O4 K1 K2 4_554 5_554 105.67(12)
O4 K1 K2 6_554 5_554 47.51(3)
O4 K1 K2 5_554 5_554 47.51(3)
O4 K1 K2 3 5_554 132.95(2)
O4 K1 K2 . 5_554 77.10(10)
O4 K1 K2 2 5_554 132.95(2)
K1 K1 K2 4_554 5_554 56.76(4)
K1 K1 K2 4 5_554 123.24(4)
Mo2 K1 K2 3 5_554 125.107(14)
Mo2 K1 K2 . 5_554 52.42(3)
Mo2 K1 K2 2 5_554 125.107(14)
K2 K1 K2 . 5_554 77.824(15)
K2 K1 K2 2 5_554 166.29(8)
K2 K1 K2 3 5_554 77.824(15)
K2 K1 K2 4_554 5_554 92.83(5)
K2 K1 K2 6_554 5_554 92.83(5)
O5 K2 O3 6_554 8 75.82(11)
O5 K2 O3 6_554 . 75.82(11)
O3 K2 O3 8 . 132.1(2)
O5 K2 O2 6_554 . 70.96(14)
O3 K2 O2 8 . 128.03(13)
O3 K2 O2 . . 75.75(12)
O5 K2 O2 6_554 3_565 70.96(14)
O3 K2 O2 8 3_565 75.75(12)
O3 K2 O2 . 3_565 128.03(13)
O2 K2 O2 . 3_565 56.29(18)
O5 K2 O3 6_554 10 140.73(10)
O3 K2 O3 8 10 139.09(16)
O3 K2 O3 . 10 84.18(9)
O2 K2 O3 . 10 71.51(13)
O2 K2 O3 3_565 10 97.20(14)
O5 K2 O3 6_554 6 140.73(10)
O3 K2 O3 8 6 84.18(9)
O3 K2 O3 . 6 139.09(16)
O2 K2 O3 . 6 97.20(14)
O2 K2 O3 3_565 6 71.51(13)
O3 K2 O3 10 6 55.93(14)
O5 K2 O4 6_554 . 122.17(14)
O3 K2 O4 8 . 114.36(12)
O3 K2 O4 . . 55.02(10)
O2 K2 O4 . . 116.99(12)
O2 K2 O4 3_565 . 164.27(17)
O3 K2 O4 10 . 67.20(12)
O3 K2 O4 6 . 96.78(13)
O5 K2 O4 6_554 2 122.17(14)
O3 K2 O4 8 2 55.01(10)
O3 K2 O4 . 2 114.36(12)
O2 K2 O4 . 2 164.27(17)
O2 K2 O4 3_565 2 116.99(12)
O3 K2 O4 10 2 96.79(13)
O3 K2 O4 6 2 67.20(12)
O4 K2 O4 . 2 65.27(15)
O5 K2 O4 6_554 6_554 53.91(12)
O3 K2 O4 8 6_554 66.07(12)
O3 K2 O4 . 6_554 66.07(12)
O2 K2 O4 . 6_554 118.02(15)
O2 K2 O4 3_565 6_554 118.02(15)
O3 K2 O4 10 6_554 143.10(8)
O3 K2 O4 6 6_554 143.10(8)
O4 K2 O4 . 6_554 77.67(10)
O4 K2 O4 2 6_554 77.67(10)
O5 K2 Mo1 6_554 . 77.06(10)
O3 K2 Mo1 8 . 105.08(9)
O3 K2 Mo1 . . 105.08(9)
O2 K2 Mo1 . . 29.37(9)
O2 K2 Mo1 3_565 . 29.37(9)
O3 K2 Mo1 10 . 76.04(9)
O3 K2 Mo1 6 . 76.04(9)
O4 K2 Mo1 . . 139.03(10)
O4 K2 Mo1 2 . 139.03(10)
O4 K2 Mo1 6_554 . 130.97(11)
O5 K2 Mo2 6_554 . 102.14(7)
O3 K2 Mo2 8 . 133.78(11)
O3 K2 Mo2 . . 27.66(7)
O2 K2 Mo2 . . 92.17(9)
O2 K2 Mo2 3_565 . 148.43(9)
O3 K2 Mo2 10 . 68.15(7)
O3 K2 Mo2 6 . 115.92(10)
O4 K2 Mo2 . . 28.71(7)
O4 K2 Mo2 2 . 93.08(8)
O4 K2 Mo2 6_554 . 75.68(5)
Mo1 K2 Mo2 . . 119.66(3)
O5 K2 Mo2 6_554 2 102.14(7)
O3 K2 Mo2 8 2 27.66(7)
O3 K2 Mo2 . 2 133.78(11)
O2 K2 Mo2 . 2 148.43(9)
O2 K2 Mo2 3_565 2 92.17(9)
O3 K2 Mo2 10 2 115.92(10)
O3 K2 Mo2 6 2 68.15(7)
O4 K2 Mo2 . 2 93.08(8)
O4 K2 Mo2 2 2 28.71(7)
O4 K2 Mo2 6_554 2 75.69(5)
Mo1 K2 Mo2 . 2 119.65(3)
Mo2 K2 Mo2 . 2 119.31(4)
O5 K2 Mo2 6_554 6 154.75(10)
O3 K2 Mo2 8 6 111.07(11)
O3 K2 Mo2 . 6 111.07(11)
O2 K2 Mo2 . 6 86.88(13)
O2 K2 Mo2 3_565 6 86.88(12)
O3 K2 Mo2 10 6 28.17(7)
O3 K2 Mo2 6 6 28.17(7)
O4 K2 Mo2 . 6 78.27(11)
O4 K2 Mo2 2 6 78.27(11)
O4 K2 Mo2 6_554 6 151.34(9)
Mo1 K2 Mo2 . 6 77.68(6)
Mo2 K2 Mo2 . 6 90.32(5)
Mo2 K2 Mo2 2 6 90.33(5)
O5 K2 Mo2 6_554 6_554 26.03(9)
O3 K2 Mo2 8 6_554 68.78(11)
O3 K2 Mo2 . 6_554 68.77(11)
O2 K2 Mo2 . 6_554 93.81(13)
O2 K2 Mo2 3_565 6_554 93.81(13)
O3 K2 Mo2 10 6_554 151.91(7)
O3 K2 Mo2 6 6_554 151.91(7)
O4 K2 Mo2 . 6_554 101.07(10)
O4 K2 Mo2 2 6_554 101.07(10)
O4 K2 Mo2 6_554 6_554 27.87(7)
Mo1 K2 Mo2 . 6_554 103.10(6)
Mo2 K2 Mo2 . 6_554 89.28(5)
Mo2 K2 Mo2 2 6_554 89.28(5)
Mo2 K2 Mo2 6 6_554 179.22(5)
O5 K2 K1 6_554 . 96.12(11)
O3 K2 K1 8 . 72.82(10)
O3 K2 K1 . . 72.82(10)
O2 K2 K1 . . 148.14(10)
O2 K2 K1 3_565 . 148.14(10)
O3 K2 K1 10 . 109.90(8)
O3 K2 K1 6 . 109.90(8)
O4 K2 K1 . . 45.13(9)
O4 K2 K1 2 . 45.13(9)
O4 K2 K1 6_554 . 42.21(8)
Mo1 K2 K1 . . 173.18(9)
Mo2 K2 K1 . . 61.37(2)
Mo2 K2 K1 2 . 61.37(2)
Mo2 K2 K1 6 . 109.13(5)
Mo2 K2 K1 6_554 . 70.08(5)
O5 K2 Ag2 6_554 4_664 51.7(4)
O3 K2 Ag2 8 4_664 127.4(4)
O3 K2 Ag2 . 4_664 38.9(3)
O2 K2 Ag2 . 4_664 43.3(3)
O2 K2 Ag2 3_565 4_664 89.2(3)
O3 K2 Ag2 10 4_664 92.1(4)
O3 K2 Ag2 6 4_664 138.3(3)
O4 K2 Ag2 . 4_664 93.2(4)
O4 K2 Ag2 2 4_664 150.8(3)
O4 K2 Ag2 6_554 4_664 78.6(3)
Mo1 K2 Ag2 . 4_664 70.2(3)
Mo2 K2 Ag2 . 4_664 64.6(3)
Mo2 K2 Ag2 2 4_664 151.5(4)
Mo2 K2 Ag2 6 4_664 118.2(3)
Mo2 K2 Ag2 6_554 4_664 62.2(3)
K1 K2 Ag2 . 4_664 105.7(3)
O5 K2 Ag2 6_554 6_554 51.7(4)
O3 K2 Ag2 8 6_554 38.9(3)
O3 K2 Ag2 . 6_554 127.4(4)
O2 K2 Ag2 . 6_554 89.2(3)
O2 K2 Ag2 3_565 6_554 43.3(3)
O3 K2 Ag2 10 6_554 138.3(3)
O3 K2 Ag2 6 6_554 92.1(4)
O4 K2 Ag2 . 6_554 150.8(3)
O4 K2 Ag2 2 6_554 93.2(4)
O4 K2 Ag2 6_554 6_554 78.6(3)
Mo1 K2 Ag2 . 6_554 70.2(3)
Mo2 K2 Ag2 . 6_554 151.5(3)
Mo2 K2 Ag2 2 6_554 64.6(3)
Mo2 K2 Ag2 6 6_554 118.2(3)
Mo2 K2 Ag2 6_554 6_554 62.2(3)
K1 K2 Ag2 . 6_554 105.7(3)
Ag2 K2 Ag2 4_664 6_554 98.5(7)
O5 K2 K3 6_554 4_664 47.00(10)
O3 K2 K3 8 4_664 122.69(16)
O3 K2 K3 . 4_664 41.52(12)
O2 K2 K3 . 4_664 44.43(13)
O2 K2 K3 3_565 4_664 87.19(15)
O3 K2 K3 10 4_664 96.59(11)
O3 K2 K3 6 4_664 140.89(11)
O4 K2 K3 . 4_664 96.30(13)
O4 K2 K3 2 4_664 150.47(13)
O4 K2 K3 6_554 4_664 75.83(10)
Mo1 K2 K3 . 4_664 70.00(9)
Mo2 K2 K3 . 4_664 67.93(10)
Mo2 K2 K3 2 4_664 147.26(12)
Mo2 K2 K3 6 4_664 122.27(9)
Mo2 K2 K3 6_554 4_664 58.16(9)
K1 K2 K3 . 4_664 105.42(9)
Ag2 K2 K3 4_664 4_664 4.7(4)
Ag2 K2 K3 6_554 4_664 94.1(3)
O5 K2 K3 6_554 6_554 47.00(10)
O3 K2 K3 8 6_554 41.52(12)
O3 K2 K3 . 6_554 122.69(16)
O2 K2 K3 . 6_554 87.19(15)
O2 K2 K3 3_565 6_554 44.43(13)
O3 K2 K3 10 6_554 140.89(11)
O3 K2 K3 6 6_554 96.59(11)
O4 K2 K3 . 6_554 150.47(13)
O4 K2 K3 2 6_554 96.30(13)
O4 K2 K3 6_554 6_554 75.83(10)
Mo1 K2 K3 . 6_554 70.00(9)
Mo2 K2 K3 . 6_554 147.26(12)
Mo2 K2 K3 2 6_554 67.93(10)
Mo2 K2 K3 6 6_554 122.28(9)
Mo2 K2 K3 6_554 6_554 58.16(9)
K1 K2 K3 . 6_554 105.42(9)
Ag2 K2 K3 4_664 6_554 94.1(3)
Ag2 K2 K3 6_554 6_554 4.7(4)
K3 K2 K3 4_664 6_554 89.7(2)
O3 K3 O3 4_665 10 111.3(3)
O3 K3 O2 4_665 . 83.6(2)
O3 K3 O2 10 . 83.6(2)
O3 K3 O2 4_665 4_665 83.23(19)
O3 K3 O2 10 4_665 83.23(19)
O2 K3 O2 . 4_665 156.6(3)
O3 K3 O5 4_665 . 153.2(3)
O3 K3 O5 10 . 75.74(13)
O2 K3 O5 . . 123.13(19)
O2 K3 O5 4_665 . 71.74(19)
O3 K3 O5 4_665 3_665 75.74(13)
O3 K3 O5 10 3_665 153.2(3)
O2 K3 O5 . 3_665 123.13(19)
O2 K3 O5 4_665 3_665 71.74(19)
O5 K3 O5 . 3_665 87.3(2)
O3 K3 Ag1 4_665 . 116.16(18)
O3 K3 Ag1 10 . 116.16(18)
O2 K3 Ag1 . . 140.0(3)
O2 K3 Ag1 4_665 . 63.41(19)
O5 K3 Ag1 . . 43.64(12)
O5 K3 Ag1 3_665 . 43.64(12)
O3 K3 O3 4_665 7_665 80.09(13)
O3 K3 O3 10 7_665 151.2(3)
O2 K3 O3 . 7_665 71.07(16)
O2 K3 O3 4_665 7_665 125.2(2)
O5 K3 O3 . 7_665 106.4(2)
O5 K3 O3 3_665 7_665 53.59(13)
Ag1 K3 O3 . 7_665 78.31(14)
O3 K3 O3 4_665 . 151.2(3)
O3 K3 O3 10 . 80.10(13)
O2 K3 O3 . . 71.07(16)
O2 K3 O3 4_665 . 125.2(2)
O5 K3 O3 . . 53.59(13)
O5 K3 O3 3_665 . 106.4(2)
Ag1 K3 O3 . . 78.31(14)
O3 K3 O3 7_665 . 78.83(18)
O3 K3 Ag2 4_665 4_664 110.52(17)
O3 K3 Ag2 10 4_664 110.52(17)
O2 K3 Ag2 . 4_664 49.7(4)
O2 K3 Ag2 4_665 4_664 153.7(3)
O5 K3 Ag2 . 4_664 89.5(3)
O5 K3 Ag2 3_665 4_664 89.5(3)
Ag1 K3 Ag2 . 4_664 90.2(4)
O3 K3 Ag2 7_665 4_664 41.87(18)
O3 K3 Ag2 . 4_664 41.87(18)
O3 K3 Mo2 4_665 3_665 70.32(10)
O3 K3 Mo2 10 3_665 178.3(2)
O2 K3 Mo2 . 3_665 95.94(15)
O2 K3 Mo2 4_665 3_665 97.72(16)
O5 K3 Mo2 . 3_665 103.2(2)
O5 K3 Mo2 3_665 3_665 27.20(9)
Ag1 K3 Mo2 . 3_665 63.19(10)
O3 K3 Mo2 7_665 3_665 27.67(6)
O3 K3 Mo2 . 3_665 98.17(16)
Ag2 K3 Mo2 4_664 3_665 68.0(2)
O3 K3 Mo2 4_665 . 178.3(2)
O3 K3 Mo2 10 . 70.32(10)
O2 K3 Mo2 . . 95.94(15)
O2 K3 Mo2 4_665 . 97.72(16)
O5 K3 Mo2 . . 27.20(9)
O5 K3 Mo2 3_665 . 103.1(2)
Ag1 K3 Mo2 . . 63.18(10)
O3 K3 Mo2 7_665 . 98.17(16)
O3 K3 Mo2 . . 27.67(6)
Ag2 K3 Mo2 4_664 . 68.0(2)
Mo2 K3 Mo2 3_665 . 108.07(16)
O3 K3 K3 4_665 4_665 61.64(18)
O3 K3 K3 10 4_665 61.64(18)
O2 K3 K3 . 4_665 111.4(3)
O2 K3 K3 4_665 4_665 45.26(17)
O5 K3 K3 . 4_665 104.1(2)
O5 K3 K3 3_665 4_665 104.1(2)
Ag1 K3 K3 . 4_665 108.7(3)
O3 K3 K3 7_665 4_665 140.46(10)
O3 K3 K3 . 4_665 140.46(10)
Ag2 K3 K3 4_664 4_665 161.09(17)
Mo2 K3 K3 3_665 4_665 120.04(12)
Mo2 K3 K3 . 4_665 120.04(12)
O3 K3 K3 4_665 4_664 109.5(2)
O3 K3 K3 10 4_664 109.5(2)
O2 K3 K3 . 4_664 47.5(2)
O2 K3 K3 4_665 4_664 155.9(4)
O5 K3 K3 . 4_664 91.1(2)
O5 K3 K3 3_665 4_664 91.1(2)
Ag1 K3 K3 . 4_664 92.5(2)
O3 K3 K3 7_665 4_664 42.60(9)
O3 K3 K3 . 4_664 42.60(9)
Ag2 K3 K3 4_664 4_664 2.2(5)
Mo2 K3 K3 3_665 4_664 69.13(11)
Mo2 K3 K3 . 4_664 69.13(11)
K3 K3 K3 4_665 4_664 158.9(5)
O3 K3 K2 4_665 4_665 45.56(11)
O3 K3 K2 10 4_665 123.7(2)
O2 K3 K2 . 4_665 126.82(12)
O2 K3 K2 4_665 4_665 49.45(8)
O5 K3 K2 . 4_665 108.4(2)
O5 K3 K2 3_665 4_665 42.92(12)
Ag1 K3 K2 . 4_665 72.73(12)
O3 K3 K2 7_665 4_665 83.60(9)
O3 K3 K2 . 4_665 148.6(2)
Ag2 K3 K2 4_664 4_665 125.42(16)
Mo2 K3 K2 3_665 4_665 57.89(6)
Mo2 K3 K2 . 4_665 134.3(2)
K3 K3 K2 4_665 4_665 63.07(11)
K3 K3 K2 4_664 4_665 126.20(11)
O3 K3 K2 4_665 5 123.7(2)
O3 K3 K2 10 5 45.56(11)
O2 K3 K2 . 5 126.82(12)
O2 K3 K2 4_665 5 49.45(8)
O5 K3 K2 . 5 42.92(12)
O5 K3 K2 3_665 5 108.4(2)
Ag1 K3 K2 . 5 72.73(12)
O3 K3 K2 7_665 5 148.6(2)
O3 K3 K2 . 5 83.60(9)
Ag2 K3 K2 4_664 5 125.42(16)
Mo2 K3 K2 3_665 5 134.3(2)
Mo2 K3 K2 . 5 57.89(6)
K3 K3 K2 4_665 5 63.07(11)
K3 K3 K2 4_664 5 126.20(11)
K2 K3 K2 4_665 5 98.90(16)
O3 K3 Mo1 4_665 . 72.85(18)
O3 K3 Mo1 10 . 72.85(18)
O2 K3 Mo1 . . 20.18(13)
O2 K3 Mo1 4_665 . 136.4(2)
O5 K3 Mo1 . . 132.59(14)
O5 K3 Mo1 3_665 . 132.59(14)
Ag1 K3 Mo1 . . 160.15(19)
O3 K3 Mo1 7_665 . 86.41(15)
O3 K3 Mo1 . . 86.41(15)
Ag2 K3 Mo1 4_664 . 69.9(3)
Mo2 K3 Mo1 3_665 . 107.25(13)
Mo2 K3 Mo1 . . 107.25(13)
K3 K3 Mo1 4_665 . 91.2(3)
K3 K3 Mo1 4_664 . 67.7(2)
K2 K3 Mo1 4_665 . 118.41(12)
K2 K3 Mo1 5 . 118.41(12)
O3 K3 Ag2 4_665 4_665 62.8(2)
O3 K3 Ag2 10 4_665 62.8(2)
O2 K3 Ag2 . 4_665 114.7(3)
O2 K3 Ag2 4_665 4_665 41.9(4)
O5 K3 Ag2 . 4_665 101.7(2)
O5 K3 Ag2 3_665 4_665 101.7(2)
Ag1 K3 Ag2 . 4_665 105.3(3)
O3 K3 Ag2 7_665 4_665 140.59(9)
O3 K3 Ag2 . 4_665 140.59(9)
Ag2 K3 Ag2 4_664 4_665 164.4(6)
Mo2 K3 Ag2 3_665 4_665 118.80(13)
Mo2 K3 Ag2 . 4_665 118.80(13)
K3 K3 Ag2 4_665 4_665 3.4(5)
K3 K3 Ag2 4_664 4_665 162.22(15)
K2 K3 Ag2 4_665 4_665 61.35(19)
K2 K3 Ag2 5 4_665 61.35(19)
Mo1 K3 Ag2 . 4_665 94.5(3)
O3 K3 K2 4_665 2_665 48.70(15)
O3 K3 K2 10 2_665 124.7(3)
O2 K3 K2 . 2_665 48.24(8)
O2 K3 K2 4_665 2_665 129.16(10)
O5 K3 K2 . 2_665 148.6(2)
O5 K3 K2 3_665 2_665 80.01(10)
Ag1 K3 K2 . 2_665 118.51(12)
O3 K3 K2 7_665 2_665 43.60(9)
O3 K3 K2 . 2_665 102.76(17)
Ag2 K3 K2 4_664 2_665 62.01(19)
Mo2 K3 K2 3_665 2_665 55.76(5)
Mo2 K3 K2 . 2_665 129.94(17)
K3 K3 K2 4_665 2_665 106.9(2)
K3 K3 K2 4_664 2_665 60.83(14)
K2 K3 K2 4_665 2_665 81.17(4)
K2 K3 K2 5 2_665 167.8(2)
Mo1 K3 K2 . 2_665 52.58(9)
Ag2 K3 K2 4_665 2_665 108.94(16)
O3 K3 K2 4_665 . 124.7(3)
O3 K3 K2 10 . 48.70(15)
O2 K3 K2 . . 48.24(8)
O2 K3 K2 4_665 . 129.16(10)
O5 K3 K2 . . 80.01(10)
O5 K3 K2 3_665 . 148.6(2)
Ag1 K3 K2 . . 118.51(12)
O3 K3 K2 7_665 . 102.76(17)
O3 K3 K2 . . 43.60(9)
Ag2 K3 K2 4_664 . 62.01(19)
Mo2 K3 K2 3_665 . 129.94(17)
Mo2 K3 K2 . . 55.76(5)
K3 K3 K2 4_665 . 106.9(2)
K3 K3 K2 4_664 . 60.83(14)
K2 K3 K2 4_665 . 167.8(2)
K2 K3 K2 5 . 81.17(4)
Mo1 K3 K2 . . 52.58(9)
Ag2 K3 K2 4_665 . 108.94(16)
K2 K3 K2 2_665 . 96.18(16)
O1 Ag1 O5 4_664 . 93.21(12)
O1 Ag1 O5 4_664 2_655 93.21(12)
O5 Ag1 O5 . 2_655 119.69(2)
O1 Ag1 O5 4_664 3_665 93.21(12)
O5 Ag1 O5 . 3_665 119.69(2)
O5 Ag1 O5 2_655 3_665 119.69(2)
O1 Ag1 O2 4_664 4_665 149.08(8)
O5 Ag1 O2 . 4_665 72.27(11)
O5 Ag1 O2 2_655 4_665 117.70(15)
O5 Ag1 O2 3_665 4_665 72.27(11)
O1 Ag1 O2 4_664 6_655 149.09(9)
O5 Ag1 O2 . 6_655 117.71(15)
O5 Ag1 O2 2_655 6_655 72.27(11)
O5 Ag1 O2 3_665 6_655 72.27(11)
O2 Ag1 O2 4_665 6_655 52.84(14)
O1 Ag1 O2 4_664 5 149.09(9)
O5 Ag1 O2 . 5 72.27(11)
O5 Ag1 O2 2_655 5 72.27(11)
O5 Ag1 O2 3_665 5 117.70(15)
O2 Ag1 O2 4_665 5 52.84(14)
O2 Ag1 O2 6_655 5 52.84(14)
O1 Ag1 K3 4_664 . 98.09(11)
O5 Ag1 K3 . . 59.859(16)
O5 Ag1 K3 2_655 . 168.69(17)
O5 Ag1 K3 3_665 . 59.859(16)
O2 Ag1 K3 4_665 . 50.99(14)
O2 Ag1 K3 6_655 . 97.67(11)
O2 Ag1 K3 5 . 97.67(11)
O1 Ag1 K3 4_664 3_665 98.10(11)
O5 Ag1 K3 . 3_665 168.69(17)
O5 Ag1 K3 2_655 3_665 59.859(16)
O5 Ag1 K3 3_665 3_665 59.859(16)
O2 Ag1 K3 4_665 3_665 97.67(11)
O2 Ag1 K3 6_655 3_665 50.99(14)
O2 Ag1 K3 5 3_665 97.67(11)
K3 Ag1 K3 . 3_665 118.05(5)
O1 Ag1 K3 4_664 2_655 98.10(11)
O5 Ag1 K3 . 2_655 59.859(16)
O5 Ag1 K3 2_655 2_655 59.859(16)
O5 Ag1 K3 3_665 2_655 168.69(17)
O2 Ag1 K3 4_665 2_655 97.67(11)
O2 Ag1 K3 6_655 2_655 97.67(11)
O2 Ag1 K3 5 2_655 50.99(14)
K3 Ag1 K3 . 2_655 118.05(5)
K3 Ag1 K3 3_665 2_655 118.05(5)
O1 Ag1 Mo1 4_664 4_665 180.0
O5 Ag1 Mo1 . 4_665 86.79(12)
O5 Ag1 Mo1 2_655 4_665 86.79(12)
O5 Ag1 Mo1 3_665 4_665 86.79(12)
O2 Ag1 Mo1 4_665 4_665 30.91(8)
O2 Ag1 Mo1 6_655 4_665 30.92(8)
O2 Ag1 Mo1 5 4_665 30.92(8)
K3 Ag1 Mo1 . 4_665 81.90(11)
K3 Ag1 Mo1 3_665 4_665 81.90(11)
K3 Ag1 Mo1 2_655 4_665 81.90(11)
O1 Ag1 Ag2 4_664 . 102.1(5)
O5 Ag1 Ag2 . . 60.01(4)
O5 Ag1 Ag2 2_655 . 164.7(5)
O5 Ag1 Ag2 3_665 . 60.01(4)
O2 Ag1 Ag2 4_665 . 47.0(5)
O2 Ag1 Ag2 6_655 . 94.1(4)
O2 Ag1 Ag2 5 . 94.1(4)
K3 Ag1 Ag2 . . 4.0(5)
K3 Ag1 Ag2 3_665 . 117.03(10)
K3 Ag1 Ag2 2_655 . 117.03(10)
Mo1 Ag1 Ag2 4_665 . 77.9(5)
O1 Ag1 Ag2 4_664 3_665 102.1(5)
O5 Ag1 Ag2 . 3_665 164.7(5)
O5 Ag1 Ag2 2_655 3_665 60.01(4)
O5 Ag1 Ag2 3_665 3_665 60.01(4)
O2 Ag1 Ag2 4_665 3_665 94.1(4)
O2 Ag1 Ag2 6_655 3_665 47.0(5)
O2 Ag1 Ag2 5 3_665 94.1(4)
K3 Ag1 Ag2 . 3_665 117.03(10)
K3 Ag1 Ag2 3_665 3_665 4.0(5)
K3 Ag1 Ag2 2_655 3_665 117.03(10)
Mo1 Ag1 Ag2 4_665 3_665 77.9(5)
Ag2 Ag1 Ag2 . 3_665 115.7(3)
O1 Ag1 Ag2 4_664 2_655 102.1(5)
O5 Ag1 Ag2 . 2_655 60.01(4)
O5 Ag1 Ag2 2_655 2_655 60.01(4)
O5 Ag1 Ag2 3_665 2_655 164.7(5)
O2 Ag1 Ag2 4_665 2_655 94.1(4)
O2 Ag1 Ag2 6_655 2_655 94.1(4)
O2 Ag1 Ag2 5 2_655 47.0(5)
K3 Ag1 Ag2 . 2_655 117.03(10)
K3 Ag1 Ag2 3_665 2_655 117.03(10)
K3 Ag1 Ag2 2_655 2_655 4.0(5)
Mo1 Ag1 Ag2 4_665 2_655 77.9(5)
Ag2 Ag1 Ag2 . 2_655 115.7(3)
Ag2 Ag1 Ag2 3_665 2_655 115.7(3)
O1 Ag1 Mo2 4_664 2_655 71.468(16)
O5 Ag1 Mo2 . 2_655 119.41(4)
O5 Ag1 Mo2 2_655 2_655 21.74(12)
O5 Ag1 Mo2 3_665 2_655 119.42(4)
O2 Ag1 Mo2 4_665 2_655 139.45(9)
O2 Ag1 Mo2 6_655 2_655 91.67(5)
O2 Ag1 Mo2 5 2_655 91.67(5)
K3 Ag1 Mo2 . 2_655 169.56(11)
K3 Ag1 Mo2 3_665 2_655 64.88(5)
K3 Ag1 Mo2 2_655 2_655 64.88(5)
Mo1 Ag1 Mo2 4_665 2_655 108.535(16)
Ag2 Ag1 Mo2 . 2_655 173.6(5)
Ag2 Ag1 Mo2 3_665 2_655 66.6(2)
Ag2 Ag1 Mo2 2_655 2_655 66.6(2)
O1 Ag1 Mo2 4_664 . 71.466(16)
O5 Ag1 Mo2 . . 21.74(12)
O5 Ag1 Mo2 2_655 . 119.41(4)
O5 Ag1 Mo2 3_665 . 119.41(4)
O2 Ag1 Mo2 4_665 . 91.67(5)
O2 Ag1 Mo2 6_655 . 139.45(9)
O2 Ag1 Mo2 5 . 91.67(5)
K3 Ag1 Mo2 . . 64.88(5)
K3 Ag1 Mo2 3_665 . 169.56(11)
K3 Ag1 Mo2 2_655 . 64.88(5)
Mo1 Ag1 Mo2 4_665 . 108.533(16)
Ag2 Ag1 Mo2 . . 66.6(2)
Ag2 Ag1 Mo2 3_665 . 173.6(5)
Ag2 Ag1 Mo2 2_655 . 66.6(2)
Mo2 Ag1 Mo2 2_655 . 110.392(16)
O1 Ag1 Mo2 4_664 3_665 71.466(17)
O5 Ag1 Mo2 . 3_665 119.41(4)
O5 Ag1 Mo2 2_655 3_665 119.42(4)
O5 Ag1 Mo2 3_665 3_665 21.74(12)
O2 Ag1 Mo2 4_665 3_665 91.67(5)
O2 Ag1 Mo2 6_655 3_665 91.67(5)
O2 Ag1 Mo2 5 3_665 139.45(9)
K3 Ag1 Mo2 . 3_665 64.88(5)
K3 Ag1 Mo2 3_665 3_665 64.88(5)
K3 Ag1 Mo2 2_655 3_665 169.56(11)
Mo1 Ag1 Mo2 4_665 3_665 108.533(16)
Ag2 Ag1 Mo2 . 3_665 66.6(2)
Ag2 Ag1 Mo2 3_665 3_665 66.6(2)
Ag2 Ag1 Mo2 2_655 3_665 173.6(5)
Mo2 Ag1 Mo2 2_655 3_665 110.393(16)
Mo2 Ag1 Mo2 . 3_665 110.392(16)
O1 Ag1 Mo1 4_664 4_664 0.0010(10)
O5 Ag1 Mo1 . 4_664 93.21(12)
O5 Ag1 Mo1 2_655 4_664 93.21(12)
O5 Ag1 Mo1 3_665 4_664 93.21(12)
O2 Ag1 Mo1 4_665 4_664 149.08(8)
O2 Ag1 Mo1 6_655 4_664 149.09(8)
O2 Ag1 Mo1 5 4_664 149.09(8)
K3 Ag1 Mo1 . 4_664 98.10(11)
K3 Ag1 Mo1 3_665 4_664 98.10(11)
K3 Ag1 Mo1 2_655 4_664 98.10(11)
Mo1 Ag1 Mo1 4_665 4_664 180.0
Ag2 Ag1 Mo1 . 4_664 102.1(5)
Ag2 Ag1 Mo1 3_665 4_664 102.1(5)
Ag2 Ag1 Mo1 2_655 4_664 102.1(5)
Mo2 Ag1 Mo1 2_655 4_664 71.467(16)
Mo2 Ag1 Mo1 . 4_664 71.466(16)
Mo2 Ag1 Mo1 3_665 4_664 71.466(16)
O1 Ag1 K2 4_664 6_655 126.39(4)
O5 Ag1 K2 . 6_655 111.63(8)
O5 Ag1 K2 2_655 6_655 33.18(12)
O5 Ag1 K2 3_665 6_655 111.63(8)
O2 Ag1 K2 4_665 6_655 84.53(9)
O2 Ag1 K2 6_655 6_655 44.29(3)
O2 Ag1 K2 5 6_655 44.29(3)
K3 Ag1 K2 . 6_655 135.52(12)
K3 Ag1 K2 3_665 6_655 61.18(7)
K3 Ag1 K2 2_655 6_655 61.18(7)
Mo1 Ag1 K2 4_665 6_655 53.61(4)
Ag2 Ag1 K2 . 6_655 131.5(5)
Ag2 Ag1 K2 3_665 6_655 58.8(3)
Ag2 Ag1 K2 2_655 6_655 58.8(3)
Mo2 Ag1 K2 2_655 6_655 54.92(3)
Mo2 Ag1 K2 . 6_655 124.764(10)
Mo2 Ag1 K2 3_665 6_655 124.765(10)
Mo1 Ag1 K2 4_664 6_655 126.39(4)
O1 Ag1 K2 4_664 4_665 126.39(4)
O5 Ag1 K2 . 4_665 111.63(8)
O5 Ag1 K2 2_655 4_665 111.63(8)
O5 Ag1 K2 3_665 4_665 33.18(12)
O2 Ag1 K2 4_665 4_665 44.29(3)
O2 Ag1 K2 6_655 4_665 44.29(3)
O2 Ag1 K2 5 4_665 84.53(9)
K3 Ag1 K2 . 4_665 61.18(7)
K3 Ag1 K2 3_665 4_665 61.18(7)
K3 Ag1 K2 2_655 4_665 135.52(12)
Mo1 Ag1 K2 4_665 4_665 53.61(4)
Ag2 Ag1 K2 . 4_665 58.8(3)
Ag2 Ag1 K2 3_665 4_665 58.8(3)
Ag2 Ag1 K2 2_655 4_665 131.5(5)
Mo2 Ag1 K2 2_655 4_665 124.765(10)
Mo2 Ag1 K2 . 4_665 124.765(9)
Mo2 Ag1 K2 3_665 4_665 54.92(3)
Mo1 Ag1 K2 4_664 4_665 126.39(4)
K2 Ag1 K2 6_655 4_665 88.40(6)
O3 Ag2 O3 4_665 10 123.8(10)
O3 Ag2 O2 4_665 4_665 88.6(7)
O3 Ag2 O2 10 4_665 88.6(7)
O3 Ag2 O2 4_665 . 86.8(7)
O3 Ag2 O2 10 . 86.8(7)
O2 Ag2 O2 4_665 . 170.3(11)
O3 Ag2 O5 4_665 . 152.3(10)
O3 Ag2 O5 10 . 74.8(3)
O2 Ag2 O5 4_665 . 70.3(6)
O2 Ag2 O5 . . 116.6(7)
O3 Ag2 O5 4_665 3_665 74.8(3)
O3 Ag2 O5 10 3_665 152.3(10)
O2 Ag2 O5 4_665 3_665 70.3(6)
O2 Ag2 O5 . 3_665 116.6(7)
O5 Ag2 O5 . 3_665 81.1(6)
O3 Ag2 K3 4_665 4_665 68.0(6)
O3 Ag2 K3 10 4_665 68.0(6)
O2 Ag2 K3 4_665 4_665 49.7(5)
O2 Ag2 K3 . 4_665 120.7(7)
O5 Ag2 K3 . 4_665 107.5(6)
O5 Ag2 K3 3_665 4_665 107.5(6)
O3 Ag2 Ag1 4_665 . 113.5(6)
O3 Ag2 Ag1 10 . 113.5(6)
O2 Ag2 Ag1 4_665 . 60.8(5)
O2 Ag2 Ag1 . . 128.9(9)
O5 Ag2 Ag1 . . 40.6(3)
O5 Ag2 Ag1 3_665 . 40.6(3)
K3 Ag2 Ag1 4_665 . 110.4(7)
O3 Ag2 Ag2 4_665 4_664 107.4(8)
O3 Ag2 Ag2 10 4_664 107.4(8)
O2 Ag2 Ag2 4_665 4_664 143.5(12)
O2 Ag2 Ag2 . 4_664 46.1(7)
O5 Ag2 Ag2 . 4_664 82.4(7)
O5 Ag2 Ag2 3_665 4_664 82.4(7)
K3 Ag2 Ag2 4_665 4_664 166.8(11)
Ag1 Ag2 Ag2 . 4_664 82.8(8)
O3 Ag2 Ag2 4_665 4_665 69.2(6)
O3 Ag2 Ag2 10 4_665 69.2(6)
O2 Ag2 Ag2 4_665 4_665 46.2(6)
O2 Ag2 Ag2 . 4_665 124.1(12)
O5 Ag2 Ag2 . 4_665 104.9(9)
O5 Ag2 Ag2 3_665 4_665 104.9(9)
K3 Ag2 Ag2 4_665 4_665 3.5(5)
Ag1 Ag2 Ag2 . 4_665 107.0(10)
Ag2 Ag2 Ag2 4_664 4_665 170.3(16)
O3 Ag2 Mo1 4_665 . 76.6(6)
O3 Ag2 Mo1 10 . 76.6(6)
O2 Ag2 Mo1 4_665 . 147.6(9)
O2 Ag2 Mo1 . . 22.7(3)
O5 Ag2 Mo1 . . 130.5(6)
O5 Ag2 Mo1 3_665 . 130.5(6)
K3 Ag2 Mo1 4_665 . 97.9(5)
Ag1 Ag2 Mo1 . . 151.6(8)
Ag2 Ag2 Mo1 4_664 . 68.9(8)
Ag2 Ag2 Mo1 4_665 . 101.4(9)
O3 Ag2 K2 4_665 4_665 46.4(3)
O3 Ag2 K2 10 4_665 132.2(10)
O2 Ag2 K2 4_665 4_665 50.5(3)
O2 Ag2 K2 . 4_665 129.0(3)
O5 Ag2 K2 . 4_665 106.1(7)
O5 Ag2 K2 3_665 4_665 43.5(2)
K3 Ag2 K2 4_665 4_665 66.3(4)
Ag1 Ag2 K2 . 4_665 71.2(4)
Ag2 Ag2 K2 4_664 4_665 120.3(5)
Ag2 Ag2 K2 4_665 4_665 64.5(5)
Mo1 Ag2 K2 . 4_665 122.9(4)
O3 Ag2 K2 4_665 5 132.2(10)
O3 Ag2 K2 10 5 46.4(3)
O2 Ag2 K2 4_665 5 50.5(3)
O2 Ag2 K2 . 5 129.0(3)
O5 Ag2 K2 . 5 43.5(2)
O5 Ag2 K2 3_665 5 106.1(7)
K3 Ag2 K2 4_665 5 66.3(4)
Ag1 Ag2 K2 . 5 71.2(4)
Ag2 Ag2 K2 4_664 5 120.3(5)
Ag2 Ag2 K2 4_665 5 64.5(5)
Mo1 Ag2 K2 . 5 122.9(4)
K2 Ag2 K2 4_665 5 101.0(6)
O3 Ag2 Mo2 4_665 3_665 67.8(3)
O3 Ag2 Mo2 10 3_665 168.0(8)
O2 Ag2 Mo2 4_665 3_665 94.8(5)
O2 Ag2 Mo2 . 3_665 91.3(6)
O5 Ag2 Mo2 . 3_665 95.5(6)
O5 Ag2 Mo2 3_665 3_665 25.47(16)
K3 Ag2 Mo2 4_665 3_665 122.6(4)
Ag1 Ag2 Mo2 . 3_665 59.1(3)
Ag2 Ag2 Mo2 4_664 3_665 63.6(4)
Ag2 Ag2 Mo2 4_665 3_665 121.1(6)
Mo1 Ag2 Mo2 . 3_665 105.6(5)
K2 Ag2 Mo2 4_665 3_665 56.84(17)
K2 Ag2 Mo2 5 3_665 129.7(7)
O3 Ag2 Mo2 4_665 . 168.0(8)
O3 Ag2 Mo2 10 . 67.8(3)
O2 Ag2 Mo2 4_665 . 94.8(5)
O2 Ag2 Mo2 . . 91.3(6)
O5 Ag2 Mo2 . . 25.47(16)
O5 Ag2 Mo2 3_665 . 95.5(6)
K3 Ag2 Mo2 4_665 . 122.6(4)
Ag1 Ag2 Mo2 . . 59.1(3)
Ag2 Ag2 Mo2 4_664 . 63.6(4)
Ag2 Ag2 Mo2 4_665 . 121.1(6)
Mo1 Ag2 Mo2 . . 105.6(5)
K2 Ag2 Mo2 4_665 . 129.7(7)
K2 Ag2 Mo2 5 . 56.84(17)
Mo2 Ag2 Mo2 3_665 . 100.3(5)
O3 Ag2 K3 4_665 4_664 106.5(7)
O3 Ag2 K3 10 4_664 106.5(7)
O2 Ag2 K3 4_665 4_664 145.9(8)
O2 Ag2 K3 . 4_664 43.8(4)
O5 Ag2 K3 . 4_664 84.1(5)
O5 Ag2 K3 3_665 4_664 84.1(5)
K3 Ag2 K3 4_665 4_664 164.4(6)
Ag1 Ag2 K3 . 4_664 85.1(5)
Ag2 Ag2 K3 4_664 4_664 2.3(5)
Ag2 Ag2 K3 4_665 4_664 167.9(11)
Mo1 Ag2 K3 . 4_664 66.5(4)
K2 Ag2 K3 4_665 4_664 121.3(4)
K2 Ag2 K3 5 4_664 121.3(4)
Mo2 Ag2 K3 3_665 4_664 64.8(4)
Mo2 Ag2 K3 . 4_664 64.8(4)
O3 Ag2 Mo2 4_665 4_665 13.4(3)
O3 Ag2 Mo2 10 4_665 110.5(8)
O2 Ag2 Mo2 4_665 4_665 89.4(5)
O2 Ag2 Mo2 . 4_665 84.2(5)
O5 Ag2 Mo2 . 4_665 159.1(9)
O5 Ag2 Mo2 3_665 4_665 87.64(17)
K3 Ag2 Mo2 4_665 4_665 59.3(3)
Ag1 Ag2 Mo2 . 4_665 124.9(4)
Ag2 Ag2 Mo2 4_664 4_665 113.7(7)
Ag2 Ag2 Mo2 4_665 4_665 61.0(4)
Mo1 Ag2 Mo2 . 4_665 69.8(4)
K2 Ag2 Mo2 4_665 4_665 54.73(18)
K2 Ag2 Mo2 5 4_665 125.5(7)
Mo2 Ag2 Mo2 3_665 4_665 81.05(3)
Mo2 Ag2 Mo2 . 4_665 175.4(8)
K3 Ag2 Mo2 4_664 4_665 112.3(4)
O3 Ag2 Mo2 4_665 6 110.5(8)
O3 Ag2 Mo2 10 6 13.4(3)
O2 Ag2 Mo2 4_665 6 89.4(5)
O2 Ag2 Mo2 . 6 84.2(5)
O5 Ag2 Mo2 . 6 87.64(17)
O5 Ag2 Mo2 3_665 6 159.1(9)
K3 Ag2 Mo2 4_665 6 59.3(3)
Ag1 Ag2 Mo2 . 6 124.9(4)
Ag2 Ag2 Mo2 4_664 6 113.7(7)
Ag2 Ag2 Mo2 4_665 6 61.0(4)
Mo1 Ag2 Mo2 . 6 69.8(4)
K2 Ag2 Mo2 4_665 6 125.5(7)
K2 Ag2 Mo2 5 6 54.73(18)
Mo2 Ag2 Mo2 3_665 6 175.4(8)
Mo2 Ag2 Mo2 . 6 81.05(3)
K3 Ag2 Mo2 4_664 6 112.3(4)
Mo2 Ag2 Mo2 4_665 6 97.2(5)
O3 Ag2 K2 4_665 2_665 48.2(4)
O3 Ag2 K2 10 2_665 129.8(9)
O2 Ag2 K2 4_665 2_665 132.0(3)
O2 Ag2 K2 . 2_665 47.9(3)
O5 Ag2 K2 . 2_665 138.6(8)
O5 Ag2 K2 3_665 2_665 77.8(3)
K3 Ag2 K2 4_665 2_665 112.6(4)
Ag1 Ag2 K2 . 2_665 112.5(5)
Ag2 Ag2 K2 4_664 2_665 60.0(5)
Ag2 Ag2 K2 4_665 2_665 114.7(6)
Mo1 Ag2 K2 . 2_665 53.2(3)
K2 Ag2 K2 4_665 2_665 81.65(4)
K2 Ag2 K2 5 2_665 176.1(7)
Mo2 Ag2 K2 3_665 2_665 54.21(19)
Mo2 Ag2 K2 . 2_665 123.5(7)
K3 Ag2 K2 4_664 2_665 58.8(3)
Mo2 Ag2 K2 4_665 2_665 53.81(18)
Mo2 Ag2 K2 6 2_665 121.4(6)
O3 Ag2 K2 4_665 . 129.8(9)
O3 Ag2 K2 10 . 48.2(4)
O2 Ag2 K2 4_665 . 132.0(3)
O2 Ag2 K2 . . 47.9(3)
O5 Ag2 K2 . . 77.8(3)
O5 Ag2 K2 3_665 . 138.6(8)
K3 Ag2 K2 4_665 . 112.6(4)
Ag1 Ag2 K2 . . 112.5(5)
Ag2 Ag2 K2 4_664 . 60.0(5)
Ag2 Ag2 K2 4_665 . 114.7(6)
Mo1 Ag2 K2 . . 53.2(3)
K2 Ag2 K2 4_665 . 176.1(7)
K2 Ag2 K2 5 . 81.65(4)
Mo2 Ag2 K2 3_665 . 123.5(7)
Mo2 Ag2 K2 . . 54.21(19)
K3 Ag2 K2 4_664 . 58.8(3)
Mo2 Ag2 K2 4_665 . 121.4(6)
Mo2 Ag2 K2 6 . 53.81(18)
K2 Ag2 K2 2_665 . 95.5(6)
Mo1 O1 Ag1 . 4_665 180.0
Mo1 O2 K3 . . 128.0(3)
Mo1 O2 Ag2 . 4_664 151.4(6)
K3 O2 Ag2 . 4_664 80.6(6)
Mo1 O2 Ag2 . . 120.9(6)
K3 O2 Ag2 . . 7.1(6)
Ag2 O2 Ag2 4_664 . 87.70(17)
Mo1 O2 K3 . 4_664 144.8(3)
K3 O2 K3 . 4_664 87.25(14)
Ag2 O2 K3 4_664 4_664 6.6(6)
Ag2 O2 K3 . 4_664 94.3(6)
Mo1 O2 K2 . 2_665 92.88(9)
K3 O2 K2 . 2_665 90.31(10)
Ag2 O2 K2 4_664 2_665 86.21(11)
Ag2 O2 K2 . 2_665 90.79(11)
K3 O2 K2 4_664 2_665 86.12(11)
Mo1 O2 K2 . . 92.88(9)
K3 O2 K2 . . 90.31(10)
Ag2 O2 K2 4_664 . 86.21(11)
Ag2 O2 K2 . . 90.79(11)
K3 O2 K2 4_664 . 86.12(11)
K2 O2 K2 2_665 . 172.2(2)
Mo1 O2 Ag1 . 4_664 79.19(18)
K3 O2 Ag1 . 4_664 152.9(2)
Ag2 O2 Ag1 4_664 4_664 72.2(5)
Ag2 O2 Ag1 . 4_664 159.9(6)
K3 O2 Ag1 4_664 4_664 65.61(19)
K2 O2 Ag1 2_665 4_664 87.95(12)
K2 O2 Ag1 . 4_664 87.95(12)
Mo2 O3 Ag2 . 4_664 147.6(6)
Mo2 O3 K3 . 4_664 153.6(2)
Ag2 O3 K3 4_664 4_664 6.4(6)
Mo2 O3 K2 . . 103.38(18)
Ag2 O3 K2 4_664 . 94.7(6)
K3 O3 K2 4_664 . 92.92(19)
Mo2 O3 K2 . 5_554 96.43(18)
Ag2 O3 K2 4_664 5_554 94.8(7)
K3 O3 K2 4_664 5_554 90.8(2)
K2 O3 K2 . 5_554 125.03(16)
Mo2 O3 K3 . . 86.7(2)
Ag2 O3 K3 4_664 . 70.1(7)
K3 O3 K3 4_664 . 75.76(13)
K2 O3 K3 . . 80.05(17)
K2 O3 K3 5_554 . 152.63(16)
Mo2 O4 K1 . 4 161.5(3)
Mo2 O4 K1 . . 113.5(2)
K1 O4 K1 4 . 84.95(12)
Mo2 O4 K2 . . 88.70(9)
K1 O4 K2 4 . 94.96(8)
K1 O4 K2 . . 79.72(9)
Mo2 O4 K2 . 3 88.70(9)
K1 O4 K2 4 3 94.96(8)
K1 O4 K2 . 3 79.72(9)
K2 O4 K2 . 3 156.2(2)
Mo2 O4 K2 . 5 84.34(17)
K1 O4 K2 4 5 77.17(13)
K1 O4 K2 . 5 162.12(17)
K2 O4 K2 . 5 101.62(10)
K2 O4 K2 3 5 101.62(10)
Mo2 O5 Ag1 . . 129.3(2)
Mo2 O5 K2 . 5 111.88(19)
Ag1 O5 K2 . 5 118.86(18)
Mo2 O5 K3 . . 104.24(15)
Ag1 O5 K3 . . 76.51(12)
K2 O5 K3 5 . 90.08(15)
Mo2 O5 K3 . 2_655 104.24(15)
Ag1 O5 K3 . 2_655 76.51(12)
K2 O5 K3 5 2_655 90.08(15)
K3 O5 K3 . 2_655 149.2(3)
Mo2 O5 Ag2 . . 106.1(5)
Ag1 O5 Ag2 . . 79.4(3)
K2 O5 Ag2 5 . 84.7(5)
K3 O5 Ag2 . . 5.4(5)
K3 O5 Ag2 2_655 . 149.0(4)
Mo2 O5 Ag2 . 2_655 106.1(5)
Ag1 O5 Ag2 . 2_655 79.4(3)
K2 O5 Ag2 5 2_655 84.7(5)
K3 O5 Ag2 . 2_655 149.0(4)
K3 O5 Ag2 2_655 2_655 5.4(5)
Ag2 O5 Ag2 . 2_655 147.9(10)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Mo1 O2 . 1.757(5)
Mo1 O2 3_565 1.757(5)
Mo1 O2 2_665 1.757(5)
Mo1 O1 . 1.786(18)
Mo1 Ag1 4_664 3.3592(12)
Mo1 K2 3_565 3.5777(15)
Mo1 K2 2_665 3.5777(15)
Mo1 K2 . 3.5777(15)
Mo1 Ag2 2_665 3.90(3)
Mo1 Ag2 3_565 3.90(3)
Mo1 Ag2 . 3.90(3)
Mo1 K3 2_665 4.016(8)
Mo2 O3 9 1.750(3)
Mo2 O3 . 1.750(3)
Mo2 O4 . 1.762(4)
Mo2 O5 . 1.774(4)
Mo2 K2 3 3.6675(7)
Mo2 K2 . 3.6675(7)
Mo2 K2 5_554 3.683(3)
Mo2 Ag1 . 3.7077(6)
Mo2 K2 5 3.751(3)
Mo2 K3 2_655 3.761(4)
Mo2 K3 . 3.761(4)
Mo2 K1 . 3.8695(8)
K1 O4 4_554 2.690(5)
K1 O4 6_554 2.690(5)
K1 O4 5_554 2.690(5)
K1 O4 3 2.812(5)
K1 O4 . 2.812(5)
K1 O4 2 2.812(5)
K1 K1 4_554 3.71690(10)
K1 K1 4 3.71690(10)
K1 K2 . 3.9046(17)
K1 K2 2 3.9046(17)
K1 K2 3 3.9046(17)
K1 K2 4_554 4.400(2)
K1 K2 6_554 4.400(2)
K1 K2 5_554 4.400(2)
K2 O5 6_554 2.709(5)
K2 O3 8 2.844(4)
K2 O3 . 2.844(4)
K2 O2 . 3.0295(13)
K2 O2 3_565 3.0296(13)
K2 O3 10 3.051(6)
K2 O3 6 3.051(6)
K2 O4 . 3.2567(17)
K2 O4 2 3.2567(17)
K2 O4 6_554 3.489(6)
K2 Ag2 4_664 3.916(18)
K2 Ag2 6_554 3.917(18)
K2 K3 4_664 3.978(5)
K2 K3 6_554 3.978(5)
K3 O3 4_665 2.640(5)
K3 O3 10 2.640(5)
K3 O2 . 2.689(9)
K3 O2 4_665 2.791(9)
K3 O5 . 2.909(6)
K3 O5 3_665 2.909(6)
K3 Ag1 . 3.271(7)
K3 O3 7_665 3.433(7)
K3 O3 . 3.433(7)
K3 Ag2 4_664 3.48(3)
K3 K3 4_665 3.781(3)
K3 K3 4_664 3.781(3)
K3 Ag2 4_665 4.02(3)
Ag1 O1 4_664 2.289(17)
Ag1 O5 . 2.321(4)
Ag1 O5 2_655 2.321(4)
Ag1 O5 3_665 2.321(4)
Ag1 O2 4_665 3.212(6)
Ag1 O2 6_655 3.212(6)
Ag1 O2 5 3.212(6)
Ag1 Ag2 . 3.50(3)
Ag1 Ag2 3_665 3.50(3)
Ag1 Ag2 2_655 3.50(3)
Ag2 O3 4_665 2.470(12)
Ag2 O3 10 2.470(12)
Ag2 O2 4_665 2.69(3)
Ag2 O2 . 2.69(3)
Ag2 O5 . 3.088(19)
Ag2 O5 3_665 3.088(19)
Ag2 Ag2 4_664 3.730(4)
Ag2 Ag2 4_665 3.730(4)
